ACI 89-S15 Shrinkage Cracking in Fully Restrained Concrete Members
Descripción: Shrinkage Cracking...
ACI STRUCTURAL JOURNAL
Title no. 89-815
Shrinkage Cracking in Fully Restrained Concrete Members
by R. lan Gilbert This paper considers the problem of cracking in fully restrained members subjected to direct tension caused by dry shrinkage. The mechanism of direct tension cracking is discussed, and some popular misconceptions concerning the behavior of restrained members are exposed. Paper presents a rational approach for the determination of the number and spacing of cracks and the average crack width in a member, which is fully restrained and subjected only to an axial restraining force caused by shrinkage. The approach is based on the principles of mechanics and is illustrated by worked examples. Predictions agree well with observed cracking in restrained members. The procedure is used to calculate the quantities of steel required for crack control in a number of practical situations. Finally, the results of the investigation are compared with the provisions for shrinkage and temperature reinforcement in the ACI Building Code (ACI 318-89) and AS 3600-1988. Keywords: cracking (fracturing); crack width and spacing; creep; deformation; reinforced concrete; serviceability; shrinkage; slabs; structural members.
In reinforced and partially prestressed concrete structures, cracking is to be expected at service loads. Cracks may be caused by the external loads, or by restraint to shrinkage and temperature variations, or by a variety of other causes. If uncontrolled, cracking may spoil the appearance of a structure or otherwise adversely affect its performance. Excessively wide cracks in floor systems and walls may often be avoided by the inclusion of strategically placed contraction (or control) joints, thereby removing some of the restraint to shrinkage and temperature movements and reducing the internal tension. When cracking does occur, to insure that crack widths remain acceptably small, adequate quantities of well-anchored reinforcement must be included at every location in the structure where significant tension is expected. The maximum crack width, which may be considered to be acceptable in a given situation, depends on the type of structure, the environment, and the consequences of excessive cracking. In corrosive and aggressive environments, some building codes and specifications recommend that crack widths do not exceed about 0.3 mm (0.012 in.). For members with one or more exposed surfaces, a maximum crack width of 0.3 mm should also provide visual acceptability. For the sheltered interior of most buildings where the concrete is ACI Structural Journal I March-April 1992
not exposed and esthetic requirements are of secondary importance, a larger crack width may be acceptable (say 0.3 to 0.5 mm). Most existing techniques for predicting crack widths involve empirical models that have been calibrated from results obtained in laboratory tests and, as such, often fail to accurately predict crack widths in actual structures. It is difficult, therefore, for a structural designer to be confident that the cracks in a structure will in fact satisfy the maximum crack width requirements of the local building code. In beams and slabs, which have been proportioned to avoid excessive deflection at service loads and which contain sufficient quantities of reinforcement to provide adequate ultimate strength and ductility, flexural crack widths are rarely a problem under normal inservice conditions, provided of course that the reinforcement bars are not spaced too widely apart. Sensible reinforcement detailing is the key to flexural crack control. It is, therefore, not usually critical if flexural crack widths are not specifically checked in design. When flexural members are also restrained at the supports, shrinkage causes a buildup of tension in the member, in addition to the bending caused by the external loads. Crack control is still not usually a problem, since shrinkage is accommodated by small increases in the widths of the numerous flexural cracks. However, for members not subjected to significant bending in which restraint is provided to the longitudinal movement caused by shrinkage and temperature changes, cracks tend to propagate over the full depth of the section. Exessively wide cracks are not uncommon. Such cracks are commonly called direct tension cracks, since they are caused by direct tension rather than by flexural tension. In fully restrained direct tension members, relatively large amounts of reinforcement are required to control load-independent cracking. The ACI Structural Journal, V. 89, No.2, March-Aprill992. Received Apr. I, 1991, and reviewed under Institute publication policies. Copyright © 1992, American Concrete Institute. All rights reserved, including the making of copies unless permission is obtained from the copyright proprietors. Pertinent discussion will be published in the January-February 1993 ACI Structural Journal if received by Sept. I, 1992.
Jan Gilbert is Professor of Civil Engineering and Head of the Department of Structural Engineering at the University of New South Wales, Sydney, Australia. His research interests are in servicability of concrete structures, and he is the author of over 80 research papers and two books in the area. Dr. Gilbert is a member of the Concrete Structures and Composite Structures Comittees of Standards Australia and he was actively engaged in the development of the Australian Standard for Concrete Structures AS 3600-1988.
minimum quantities of reinforcement specified in the Australian Code AS 3600-1988 1 for crack control in restrained members are much greater than that required in the ACI Building Code (metric version) ACI 318M892 and are based on Australian research by Base and Murray3•4 and others. In this paper, the mechanism of direct tension cracking is discussed, and a rational approach is presented for the determination of the average crack width in a member that is fully restrained and subjected only to an axial restraining force caused by shrinkage. The predicted number and width of shrinkage cracks agree well with observed cracking in restrained members. The approach is used to calculate the quantities of steel required for crack control in restrained members for a variety of situations. Finally, the results of the investigation are compared with the provisions for crack control in AS 3600-1988 1 and ACI 318M-89. 2 CRACKING IN DIRECT TENSION MEMBERS
Consider a reinforced concrete direct tension member that is prevented from shortening by its supports or by adjacent parts of the structure. As the concrete shrinks, an axial tensile restraining force N(t) develops with time. When the concrete stress caused by N(t) at a A 5 = area of reinforcing steel (
= area of concrete
1--------L-----(a) Just prior to first cracking.
1--------L-------1 (b) Just after first cracking.
(c) Average concrete stress just after flrst cracking.
(d) Steel stress just after first cracking.
Fig. 1 - First cracking 'in a restrained direct tension member 142
particular cross section first reaches the direct (uniaxial) tensile strength of concrete j,, full-depth direct tension cracking occurs. First cracking may occur less than 1 week a£ter the commencement of drying. The magnitude of N(t) after cracking and the crack width depend primarily on the amount of bonded reinforcement crossing the crack. If the member contains no longitudinal steel, cracking causes the restraining force N(t) to drop to zero and a wide, unsightly crack results. If the member contains only small quantities of reinforcement (p = A/bh is less than about 0.003 for ,[y = 400 MPa), the steel at the crack yields (either immed~ately or after additional shrinkage), the crack opens widely, and the restraining force drops to a value of AJy, which may be only a small fraction of its value prior to cracking. If the member contains relatively large quantities of reinforcement (p greater than about 0.01 for /y = 400 MPa), the steel at each crack does not yield, the crack width remains small, and because the loss of member stiffness at cracking is not great, the restraining force remains high. Members containing large quanities of steel are therefore likely eventually to suffer many cracks, but each will be fine and well controlled. For intermediate steel quanities (0.003 < P < 0.01 when JY = 400 MPa), cracking causes a loss of stiffness, a reduction of N(t), and a crack width that may or may not be acceptable. In addition to the quantity of steel, the width of a crack in a restrained member depends on the quality of bond between the concrete and the steel, the size and distribution of the individual reinforcement bars, the concrete quality, and whether or not the axial restraining force is accompanied by bending. Direct tension cracks are more parallel-sided than flexural cracks, and hence the observed crack width is less dependent on the amount of concrete cover. FIRST CRACKING Description and notation
Consider the fully restrained member shown in Fig. 1(a). As the concrete shrinks, the restraining force N(t) gradually increases until the first crack occurs when N(t) = Acfr· Immediately after first cracking, the restraining force reduces to Nero and the concrete stress away from the crack is less than the tensile strength of the concrete j,. The concrete on either side of the crack shortens elastically and the crack opens to a width w, as shown in Fig. 1(b). At the crack, the steel carries the entire force Nero and the stress in the concrete is obviously zero. In the region immediately adjacent to the crack, the concrete and steel stresses vary considerably, and there exists a region of partial bond breakdown. At some distance S 0 on each side of the crack, the concrete and steel stresses are no longer influenced directly by the presence of the crack, as shown in Fig. l(c) and (d). In Region 1, where the distance x from the crack is greater than or equal to S 0 , the concrete and steel stresses are ac1 and ' is the final creep coefficient (defined as the ratio of the final creep strain to elastic strain under the average sustained stress u.v>· In this study, it is assumed that (19)
Fig. 4 - Concrete stress history in uncracked Region 1
The compatibility requirement is that the concrete and steel strains are identical
and using Eq. (21)
The magnitude of the final creep coefficient cJ>' is usually between 2 and 4, depending on the age at the commencement of drying and the quality of the concrete. e;h is the final shrinkage strain and depends on the relative humidity, the size and shape of the member, and the characteristics of the concrete mix. Numerical estimates of cJ>' and e;h can be obtained from ACI 2091i and elsewhere. A number of the more well-known methods for predicting both q,• and e;h have been presented and compared previously by the author. Eq. (20) may be expressed as (21) where E; is final effective modulus for concrete and is given by
In Region 1, at any distance from a crack greater than S 0 , equilibrium requires that the sum of the force in the concrete and the force in the steel is equal to N(oo). That is
Substituting Eq. (15) and (17) into Eq. (24) and rearranging gives
The final concrete strain in Region 1 is the sum of the elastic, creep, and shrinkage components and may be approximated by
where n* = E/E;. The crack spacing s (=Lim) must be first determined to calculate C2 [as defined in Eq. (16)]. Knowing that u;1 must be less than the tensile strength of concrete j, and making use of Eq. (15) and (17), Eq. (23) becomes (26) Substituting Eq. (16) and (25) into Eq. (26) gives
2 S 0 (1
The number of cracks m ( = Lis) may be taken as the smallest integer that causes Eq. (27) to be satisfied. With m thus determined, the restraining force N( oo) can be calculated using Eq. (25) and the steel and concrete stresses in the various regions of the member may be determined from Eq. (15), 17, and (23). The overall shortening of the concrete is an estimate of the sum of the crack widths. The final concrete strain at any point in Region 1 of Fig. 3 is given by Eq. (21), and in Region 2, the final concrete strain is (29)
(23) ACI Structural Journal I March-April1992
where fn varies beween zero at a crack and unity at S from a crack. If a parabolic variation of stress is as0
sumed in Region 2, the following expression for the average crack width w is obtained by integrating the concrete strain over the length of the member (30) The preceding analysis may be used to determine the number and width of shrinkage cracks, provided the assumption of linear-elastic behavior in the steel is valid. However, if the area of steel As is small, yielding may occur at each crack and the value of N( oo ), calculated from Eq. (12), will not be correct. In such a case, oo; is equal to the yield stress of the reinforcement ,[y and N( oo) is equal to ,[y As. From Eq. (23), the stress in the concrete away from the crack in Region 1 is now
the slab (As = 750 mm 2/m). The concrete cover to the reinforcement is 30 mm. Estimate the spacing s and final average width w of the restrained shrinkage cracks. Take ¢'
= 2.5; E;h = - 600 x 10- 6 ; .t; = 2.0 MPa; Ec
= 25,000 MPa; Es = 200,000 MPa; n = 8; and,[y = 400 MPa.
The concrete area and reinforcement ratio are 2
Ac ::::: Agross = 150,000 mm /m;
u' ~ (L - w)
u' 2 51 -
= As A = 0.005 c
and from Eq. (1)
(31) After the steel at the first crack yields, the tensile concrete stress